FSC 9310 JCP K20
25% INDEX, WHITE AND COLORED
Index Paper February 1, 1999
Use information: This paragraph is informational only and is not exclusively definitive of the end use.
For high quality face and back offset printing of card indexes, identification cards, office forms, notices, posters, covers, etc., requiring
execution with pen and ink, erasing quality, and above average permanence. Printed matter may include text, line illustrations, halftones,
and solid reverses.
Stock: Not less than 25 pct cotton or linen fibers; the remainder Erasing quality: Paper shall retain good ruling, writing, and typ-
bleached chemical woodpulp. ing quality, texture, and surface appearance, without ink
Note: 1 Postconsumer fiber, in any percentage, is encouraged, spreading after repeated erasures. Samples from the delivery
provided that the requirements of this Standard are met. shall show no greater resistance than the standard sample to re-
Acidity: pH value shall average not less than 6.5 for white and moval by abrasion of typewritten characters.
5.0 for colored paper. General appearance: Paper shall conform to the standard sam-
Rosin: Average, not to exceed 2.5 pct for papers having pH value ple(s) adopted by the Government.
less than 6.5.
Color: The paper in the order (or publication) shall be uniform
Grammage (g/m 2) ...................... 165 200 255 305 with a target brightness of 80 pct for the white paper. The color
Basis weight: 251⁄2 by 301⁄2 variation shall not exceed DE(CIELAB)=1.0.
inches, 500 sheets (pounds) ..... 90 110 140 170 For colored stock, paper shall match one of the established
A tolerance of ±10 pct shall be allowed. standards. Standards are blue, buff, green, pink, salmon, or yel-
Bursting strength: Average, low. Colors shall not fade and shall appear even and uniform on
not less than (kPa) ................... 270 450 580 690 the surface of the sheet. Stock shall not be 2-sided. Color coordi-
Equivalent (lb/in2) .................... 40 66 85 100 nates for selected standards are included in Part 3.
Thickness: Average (mm) .......... 0.190 0.230 0.290 0.350 Finish and formation: Shall be uniform.
Equivalent (inch) ...................... 0.0074 0.0091 0.0114 0.0138
A tolerance of ±0.013 mm (0.0005 inch) shall be allowed for Cleanliness: The dirt count for each side of the paper shall not
the 165, 200, 255 g/m2 paper and ±0.020 mm (0.0008 inch) on exceed 250 specks per square meter. No sample sheet (600 to
the 305 g/m2. Paper shall be uniform and shall not vary more 650 cm2 in size) shall contain more than one defect with an
than 0.011 mm (0.0004 inch) from one edge to the other. equivalent area of 0.25 mm2 or greater.
Ruling and writing qualities: Lines ruled and characters writ- Sampling and testing: Shall be conducted in accordance with
ten with pen and ink shall be clear cut and free from excessive standards in Part 2, Government Paper Specification Standards.
Unless otherwise specified, the following is automatically waived when printing or duplicating is to be accomplished on commercial contract
Sizing: Paper shall be surface- and internal-sized suitable for sat- Surface: Shall be free from lint, fuzz, or any particles which will
isfactory printing on both sides of the paper on high-speed offset pick, lift, fluff, or pile on the blanket under normal press condi-
presses equipped with continuous flow or brush dampening sys- tions.
tems. Size and trim: Sheets: Paper shall be furnished in the size(s) or-
Color: Shall match the Government’s standard sample for color. dered and shall be flat, trimmed square on four sides with clean
A deviation of DE(CIELAB)±3.0 from the color standard for smooth edges, and evenly jogged. A tolerance of ±2 mm (1⁄16
white and 2.0 for colored stocks is allowed. A color difference 1.0 inch) shall be allowed except for sheets 216 by 356 mm (81⁄2 by
DE unit between felt and wire sides is permitted. 14 inches) or less; then a tolerance of ±1 mm (1⁄32 inch) shall be
allowed. Successive sheets within any package shall not differ
For information only, the CIELAB values (Ill D65, 10° ob- from each other by more than 0.5 mm (1⁄64 inch). Paper with the
server) of the color standard are long dimension 813 mm (32 inches) or less shall be considered
L*=94.0 square if the variation does not exceed 1 mm (1⁄32 inch); over
a*=¥0.5 813 mm (32 inches), 2 mm (1⁄16 inch).
b*=4.0 Grain: Direction of the grain on flat paper shall be as ordered.
Curl: Paper shall lie flat with either no tendency to curl or with Pressroom conditions: The bulk of this paper will be used in
a curl which can be overcome under reasonable working condi- air-conditioned pressrooms maintained at 24 °C ±2 °C and 45 pct
tions. ±8 pct relative humidity.
1 This grade is typically a low Government usage paper and currently not readily and/or economically available with postconsumer
recovered fiber content. If a postconsumer recovered fiber content is desired in the paper, that number will be stated in the procurement
document. Note, recovered material (cotton/linen) is not a postconsumer recovered fiber.